Download presentation

Presentation is loading. Please wait.

Published byIsaias Longyear Modified over 3 years ago

1
UTA Noise and Reliability Laboratory 1 Noise Modeling at Quantum Level for Multi- Stack Gate Dielectric MOSFETs. Zeynep Çelik-Butler Industrial Liaisons: Ajit Shanware, Luigi Colombo, Keith Green, TI; Hsing-Huang Tseng, SEMATECH, Ania Zlotnicka, Freescale Students: Bigang Min, Siva Prasad Devireddy, Tanvir Morshed, Shahriar Rahman University of Texas at Arlington P. O. BOX 19072 Arlington, TX 76019

2
UTA Noise and Reliability Laboratory 2 Outline Noise Modeling Unified Flicker Noise Model Multi-Stack Unified Noise Model (MSUN) Experimental Verification Metal-Gated HfO 2 /SiO 2 NMOSFETs – different interfacial layer processing Poly-Gated HfSiON/SiON NMOSFETs – variable interfacial layer thickness Conclusions and Future Work

3
UTA Noise and Reliability Laboratory 3 Unified Flicker Noise Model * Based on correlated number and mobility fluctuations theory. Equi-energy tunneling process. Traps in the gate dielectric trap/de-trap channel carriers Trapping/de-trapping phenomenon causes fluctuations in the carrier number. Fluctuations in carrier mobility due to remote Coulomb scattering from trapped charge. Uniform distribution of traps in the gate dielectric with respect to distance and energy level. *K. K. Hung, P. K. Ko, C. Hu, Y. C. Cheng, “A unified model for the flicker noise in metal-oxide-semiconductor field-effect transistors,” IEEE Trans. Electron Devices, vol. 37, pp.654-665, 1990.

4
UTA Noise and Reliability Laboratory 4 Physical Mechanism for Noise Channel carriers tunnel back and forth from the traps in the gate oxide causing fluctuations in the number of carriers. By virtue of Coulomb scattering from oxide trapped charges there are fluctuations in carrier mobility that cause additional noise in correlation with the carrier number fluctuations. L z x y WSiO 2 T ox SourceDrain Substrate Traps Carriers K. K. Hung, P. K. Ko, C. Hu, Y. C. Cheng, “A unified model for the flicker noise in metal-oxide-semiconductor field-effect transistors,” IEEE Trans. Electron Devices, vol. 37, pp.654-665, 1990.

5
UTA Noise and Reliability Laboratory 5 Unified Flicker Noise Model Expressions K. K. Hung, P. K. Ko, C. Hu, and Y. C. Cheng IEEE Trans. Electron Devices, vol. 37, pp.654-665,1990 BSIM Low Frequency Noise Model

6
UTA Noise and Reliability Laboratory 6 High-k Gate Stack Scenario L z x y WHigh-k T HK T IL SourceDrain Substrate Interfacial layer Traps xx Carriers yy zz Channel carriers tunnel into the traps in high-k and interfacial layer causing fluctuations in carrier number and mobility in a correlated way. The different trap profiles and various physical properties of high- k/interfacial layer materials like physical thicknesses, barrier heights etc. affect the 1/f noise. The uniform dielectric trap density assumption does not hold.

7
UTA Noise and Reliability Laboratory 7 Multi-Stack Unified Noise Model (MSUN) Based on correlated number and mobility fluctuations theory Equi-energy tunneling process Traps in the gate dielectric layers trap/de-trap channel carriers Trapping/de-trapping phenomenon causes fluctuations in the carrier number Fluctuations in carrier mobility due to remote Coulomb scattering from trapped charge Scalable with regards to the high-k/interfacial layer physical thicknesses Takes different dielectric material properties into account Considers non-uniform distribution of traps in the high- k/interfacial layer with respect to distance and energy level

8
UTA Noise and Reliability Laboratory 8 Typical Band Diagram for High-k Stack Carrier tunneling probability into the gate dielectric is an exponentially decaying function with attenuation rates corresponding to the dielectric material. N tIL0 – IL/Si interface trap density at intrinsic Fermi level N tHK0 – HK/IL interface trap density at intrinsic Fermi level T HK EvEv E fn T IL EcEc EiEi N tIL0 N tHK0 exp[-γ HK (zT IL )] exp(-γ IL z)

9
UTA Noise and Reliability Laboratory 9 Trap Density Profile in SiO 2 01.2EiEi N t0 N t0 exp( ξ (E fn -E i )) 0z N t (E fn ) N t (E fn ) exp(ηz) Z. Çelik-Butler, and T. Y. Hsiang, “Spectral dependence of 1/f γ noise on gate bias in n-MOSFETs,” Solid State Electron., vol. 30, pp. 419–423, 1987. N t0 is the trap density at the Si/SiO 2 interface and intrinsic Fermi level. Trap density increases exponentially towards the band edges at a rate defined by parameter ξ. N t (E fn ) is the trap density at the Si/SiO 2 interface and quasi-Fermi level. Trap density increases exponentially into the gate dielectric. N t0 exp(ξ(E fn -E i )) =N t (E fn )

10
UTA Noise and Reliability Laboratory 10 Modified Trap Profile by Energy Band Bending The energy bands bend in both high-k and interfacial layers due to the applied gate voltage. Higher trap density towards the band edges means that the trap profile encountered by channel carriers at a particular location in the dielectric is altered due to band bending. This effect is reflected by the parameters λ IL and λ HK. High-K EvEv EiEi Interfacial Layer EcEc EfEf N tIL0 N tHK0 Z. Çelik-Butler, and T. Y. Hsiang, “Spectral dependence of 1/f γ noise on gate bias in n-MOSFETs,” Solid State Electron., vol. 30, pp. 419–423, 1987.

11
UTA Noise and Reliability Laboratory 11 Trap Density in High-k Stack Trap density for (0

12
UTA Noise and Reliability Laboratory 12 Total Noise Power spectral density of the mean square fluctuations in the number of occupied traps for high-k/interfacial layer stack B. Min, S. P. Devireddy, Z. Çelik-Butler, A. Shanware, L. Colombo, K. Green, J. J. Chambers, M. R. Visokay, and A. L. P. Rotondaro, “Impact of interfacial layer on low-frequency noise of HfSiON dielectric MOSFETs,” IEEE Trans. Electron Devices, vol. 53, pp. 1459–1466, 2006. Z. Çelik-Butler, “Different noise mechanisms in high-k dielectric gate stacks,” in Proc. SPIE—Noise and Fluctuations, pp. 177–184, 2005.

13
UTA Noise and Reliability Laboratory 13 MSUN Noise Model Simplification f t (1-f t ) ensures that only traps within few kT of E fn contribute to fluctuations. Integral along the channel (x) approximated. The shape of the spectral density is modified from pure 1/f through functional form of N t. Contribution to fluctuations from the high-k dielectric layer is much higher than that from the interfacial layer.

14
UTA Noise and Reliability Laboratory 14 MSUN Noise Model Expressions After appropriate substitution of various parameters, the power spectral density of the mean square fluctuations can be written as Conduction Band Offset with Si Tunneling Coefficients

15
UTA Noise and Reliability Laboratory 15 MSUN Model Expressions (con.) Total noise power spectral density Power spectral density for local current fluctuations

16
UTA Noise and Reliability Laboratory 16 Outline Noise Modeling Unified Flicker Noise Model Multi-Stack Unified Noise Model (MSUN) Experimental Verification Metal-Gated HfO 2 /SiO 2 NMOSFETs – different interfacial layer processing Poly-Gated HfSiON/SiON NMOSFETs – variable interfacial layer thickness Conclusions and Future Work

17
UTA Noise and Reliability Laboratory 17 Experimental Verification Split C-V and DC Measurements 10µm 10µm devices 78K & 100K – 350K in steps of 25K (metal gate) 172K – 300K (poly gate) Noise and DC Measurements Metal gate 0.165µm 10µm devices 78K & 100K – 350K in steps of 25K Poly gate (0.20-0.25)µm 10µm devices 172K – 300K Noise Modeling and Analysis Unified Flicker Noise Model Multi-Stack Unified Model

18
UTA Noise and Reliability Laboratory 18 Metal Gated HfO 2 /SiO 2 MOSFETs Gate Electrode High-kIL TypeIL Thickness TaSiN 27Å HfO 2 (ALD) SRPO SiO 2 10Å TaSiN 27Å HfO 2 (ALD) RCA SiO 2 10Å

19
UTA Noise and Reliability Laboratory 19 Normalized Noise vs. Temperature Normalized noise for the two process splits shows no clear dependence on temperature at all bias points. Generally, the magnitude of 10Å SRPO device is lower. Metal-Gated HfO 2 /SiO 2

20
UTA Noise and Reliability Laboratory 20 Parameter Extraction The frequency exponent for the 1-100Hz region is plotted against the applied gate bias. A straight line fit is made to the data from which η HK,λ HK are extracted The dependence of noise power spectral density on frequency mainly comes from the term, where, Metal-Gated HfO 2 /SiO 2

21
UTA Noise and Reliability Laboratory 21 Energy Dependence of Trap Density The trap density variation with respect to energy is represented as an exponentially varying function. The energy interval swept by the quasi Fermi level for the temperature and the bias range considered in this work is 0.05eV. Metal-Gated HfO 2 /SiO 2

22
UTA Noise and Reliability Laboratory 22 MSUN Model Metal-Gated HfO 2 /SiO 2

23
UTA Noise and Reliability Laboratory 23 MSUN Model Metal-Gated HfO 2 /SiO 2

24
UTA Noise and Reliability Laboratory 24 Effective Oxide Trap Density vs. Temperature N t0HK is constant for all temperatures and the non-uniformity in trap density is modeled by η HK,λ HK Metal-Gated HfO 2 /SiO 2 MSUN Model

25
UTA Noise and Reliability Laboratory 25 Effective Oxide Trap Density vs. Temperature The overall effective trap density (N t ) is extracted using the Unified Flicker Noise Model. In general, the values tend to increase with a decrease in temperature. This is not consistent with the uniform trap density assumption at the core of the model. Metal-Gated HfO 2 /SiO 2 Original Unified Noise Model

26
UTA Noise and Reliability Laboratory 26 Outline Noise Modeling Unified Flicker Noise Model Multi-Stack Unified Noise Model (MSUN) Experimental Verification Metal-Gated HfO 2 /SiO 2 NMOSFETs – different interfacial layer processing Poly-Gated HfSiON/SiON NMOSFETs – variable interfacial layer thickness Conclusions and Future Work

27
UTA Noise and Reliability Laboratory 27 Poly Gated HfSiON/SiON MOSFETs NMOS HfSiON with same high-k thickness (3.0 nm) and different interfacial layers (IL) DielectricsEOT (nm)IL (nm)Length (μm) Width (μm) Variable temperature 1/f noise measurement has been done. HfSiON1.240.80.2010 HfSiON 1.331.00.20,0.2510 HfSiON 1.461.50.20,0.2510 HfSiON 1.661.80.14 ~ 0.2510

28
UTA Noise and Reliability Laboratory 28 Temperature Dependence of Low Frequency Noise Spectral Density Normalized current noise spectral density did not show any noticeable dependence on temperature. The observed noise behavior is not affected by any temperature sensitive process. Remote optical phonon scattering may not have a significant impact on low frequency noise characteristics although it has a profound effect on mobility behavior (presented last year). Poly-Gated HfSiON / SiON

29
UTA Noise and Reliability Laboratory 29 Low Frequency Noise Mechanism Correlated Number and Mobility Fluctuation Model 1 : Hooge’s Bulk Mobility Fluctuation Model 9 : Correlated number and surface mobility fluctuation mechanism was observed to dominate for devices with different interfacial layer thicknesses in the experimental temperature range 9 F.N. Hooge. IEEE Trans. Electron Devices 41. 1926 (1994). Poly-Gated HfSiON / SiON

30
UTA Noise and Reliability Laboratory 30 The MSUN Model According to original Unified Model, current noise spectral density can be shown as Considering tunneling through a double step barrier, we can show The final expression of S id (A 2 /Hz) using the new model for high-k gate devices becomes (1) (2) (3)

31
UTA Noise and Reliability Laboratory 31 MSUN Model Parameter List High-k dielectric layer parametersInterfacial layer parameters N tHK0 Mid-gap trap density at the IL/high-k interface N tIL0 Mid-gap trap density at the substrate/IL interface μ c0 Mobility fluctuation coefficientμ c0 Mobility fluctuation coefficient λ HK Band bending parameter corresponding to the high-k layer λ IL Band bending parameter corresponding to the IL η HK Spatial trap distribution parameter for the high-k layer η IL Spatial trap distribution parameter for the interfacial layer ξ HK Parameter for the energy distribution of traps in the high-k dielectric layer ξ IL Parameter for the energy distribution of traps in the interfacial layer If the published trap density values are chosen for N tIL0 and N tHK0 the noise contribution of the interfacial layer is insignificant when compared to the total device noise. The interfacial layer parameters do not play any effective role in the data fitting For the high-k layer, as discussed earlier, λ HK = ξ HK, so the number of effective fitting parameters reduce to 4.

32
UTA Noise and Reliability Laboratory 32 Extracted ξ, λ, η From Eq (3) we can show α = From a linear fit of α as a function of V g for individual devices at all temperatures, the energy dependence parameters ξ, λ and the spatial distribution parameter η were extracted. The extracted values are shown on the plots. Poly-Gated HfSiON / SiON

33
UTA Noise and Reliability Laboratory 33 Data Vs MSUN Model Predictions for LF Noise Spectra The calculated current noise spectral density S Id is compared to the data for devices with four different IL thicknesses and in the experimental temperature range of 172K-300K. Poly-Gated HfSiON / SiON

34
UTA Noise and Reliability Laboratory 34 Data Vs MSUN Model Predictions for LF Noise Spectra Excellent agreement between data and model predictions was observed irrespective of IL thickness at all temperatures. Poly-Gated HfSiON / SiON

35
UTA Noise and Reliability Laboratory 35 Data Vs MSUN Model Predictions for LF Noise Spectra A special phenomena was observed for the devices with the thickest gate oxide. The higher frequency components in the device noise are contributed by traps closer to the interface, where as the traps further away contribute to the lower frequency components. For the devices with T IL =1.8nm, the characteristic corner frequency was calculated to be f c2 ~ 33Hz. Below 33 Hz the noise was contributed by the high-k layer. Above this limit noise contribution was primarily from the IL layer. Frequency (Hz) S Id (A 2 /Hz) α=0 α~1 α~2

36
UTA Noise and Reliability Laboratory 36 Data Vs MSUN Model Predictions for Bias Dependence The fit was good in the bias range of moderate inversion to strong inversion, for devices with all different IL thick- nesses in the experimental temperature range. Poly-Gated HfSiON / SiON

37
UTA Noise and Reliability Laboratory 37 Extracted MSUN Model Parameters EOT=1.28nm, λ HK =ξ HK =1.538eV -1, η HK =-7.99x10 6 cm -1 EOT=1.33nm, λ HK =ξ HK =-0.4056eV -1, η HK =-5.38x10 6 cm -1 T(K)N tHK0 (cm -3 eV -1 ) μ c0 (cm/Vs)T(K)N tHK0 (cm -3 eV -1 ) μ c0 (cm/Vs) 1721.7x10 19 5.0x10 10 1726.4x10 19 1.1x10 10 1881.8x10 19 5.0x10 10 1886.1x10 19 3.0x10 10 2071.7x10 19 3.0x10 10 2075.6x10 19 4.5x10 10 2301.9x10 19 2.75x10 10 2305.9x10 19 3.5x10 10 2611.4x10 19 5.0x10 10 2613.6x10 19 1.7x10 10 3001.3x10 19 5.0x10 10 3003.0x10 19 5.0x10 10 EOT=1.46nm, λ HK =ξ HK = -0.455eV -1, η HK =-4.67x10 6 cm -1 EOT=1.66nm, λ HK =ξ HK = -0.947eV -1, η HK =-3.53x10 6 cm -1 T(K)N tHK0 (cm -3 eV -1 ) μ c0 (cm/Vs)T(K)N tHK0 (cm -3 eV -1 ) μ c0 (cm/Vs) 1723.8x10 19 5.0x10 10 1722.6x10 19 5.0x10 10 1883.1x10 19 5.0x10 10 1882.3x10 19 5.0x10 10 2072.4x10 19 5.0x10 10 2071.4x10 19 7.5x10 10 2301.5x10 19 2.25x10 10 2301.6x10 19 5.0x10 10 2611.9x10 19 5.0x10 10 2501.6x10 19 5.0x10 10 3001.6x10 19 2.5x10 10 2709.0x10 18 3.0x10 10 3006.0x10 18 1.75x10 10 Poly-Gated HfSiON / SiON

38
UTA Noise and Reliability Laboratory 38 Extracted N tHK0 N tHK0 values extracted using the MSUN Model Shows consistency over the whole experimental temperature range Shows consistency with devices having different IL thickness Poly-Gated HfSiON / SiON

39
UTA Noise and Reliability Laboratory 39 Dependence of N tHK on Energy The active trap densities as probed by the quasi-Fermi energy and it’s excursion is shown for devices with different IL thicknesses. As the excursion range is comparatively small, the calculated trap density out- side the highlighted region may not correctly represent actual device characteristics. At 300K, the active trap density was observed to be IL dependent. The thinnest gate oxide devices showed highest active trap density. Poly-Gated HfSiON / SiON

40
UTA Noise and Reliability Laboratory 40 Results I The temperature dependence of extracted trap density is inconsistent with the core model assumption. Multi-Stack Unified Noise (MSUN) model is proposed to predict noise in high-k/interfacial layer MOSFETs. It is scalable with respect to HK/IL thicknesses, temperature and applied bias. It accounts for the material properties of constituent dielectric materials and the non-uniform dielectric trap density profile with respect to energy and location in dielectric. Four model parameters Mid-gap trap density at the IL/high-k interface Parameter for the energy distribution of traps in the high-k dielectric layer Spatial trap distribution parameter for the high-k layer Mobility fluctuation coefficient

41
UTA Noise and Reliability Laboratory 41 Results II The model is in excellent agreement with the experimental data down to cryogenic temperatures. Metal-Gated HfO 2 /SiO 2 NMOSFETs – different interfacial layer processing Poly-Gated HfSiON/SiON NMOSFETs – variable interfacial layer thickness Metal-Gated HfSiON/SiON MOSFETs – different nitridation techniques

42
UTA Noise and Reliability Laboratory 42 Acknowledgements Thanks to Luigi Colombo, Texas Instruments Keith Green, Texas Instruments Ajit Shanware, Texas Instruments Hsing-Huang Tseng, Freescale Ania Zlotnicka, Freescale Manuel Quevedo-Lopez, Texas Instruments / SEMATECH

Similar presentations

Presentation is loading. Please wait....

OK

Section 12: Intro to Devices

Section 12: Intro to Devices

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Download ppt on zener diode Ppt on teacher's day Ppt on seven segment display logic Ppt on review of literature example Ppt on diode characteristics conclusion Ppt on great monuments of india Ppt on resources and development class 10 cbse all 10 Ppt on carburetor systems Ppt on latest technology in electrical engineering Ppt on digital media